General

Property | Value | Condition |
---|---|---|

Density | 2.7 g/cm³ Show Material materials with Density of 2.7 g/cm³ | H32 |

2.69 g/cm³ Show Material materials with Density of 2.69 g/cm³ | H32 |

Mechanical

Property | Temperature | Value | Condition | Related Standards | Comment |
---|---|---|---|---|---|

Compressive modulus | 71.0 MPa Show Material materials with Compressive modulus of 71.0 MPa | H32 | |||

Elastic modulus | 71.0 GPa Show Material materials with Elastic modulus of 71.0 GPa | H32 | |||

70 GPa Show Material materials with Elastic modulus of 70 GPa | H32 | ||||

Elongation | 10.0 % Show Material materials with Elongation of 10.0 % | H32 | AA Standards | A50 | |

8.0 % Show Material materials with Elongation of 8.0 % | H32 | AA Standards, ASTM B209, ASTM B547 | A50 | ||

6.0 % Show Material materials with Elongation of 6.0 % | H32 | AA Standards, ASTM B209 | A50 | ||

12.0 % Show Material materials with Elongation of 12.0 % | H32 | AA Standards, ASTM B209, ASTM B547 | A50 | ||

5.0 % Show Material materials with Elongation of 5.0 % | H32 | AA Standards, ASTM B209 | A50 | ||

10.0 % Show Material materials with Elongation of 10.0 % | H32 | AA Standards, ASTM B209 | A100 | ||

5.0 % Show Material materials with Elongation of 5.0 % | H32 | AA Standards, ASTM B234 | A100 | ||

8.0 % Show Material materials with Elongation of 8.0 % | H32 | AA Standards, ASTM B234 | A100 | ||

7.9 % Show Material materials with Elongation of 7.9 % | H32 | ||||

370 °C | 130 % Show Material materials with Elongation of 130 % | H32 | Elongation in 50 mm | ||

315 °C | 110 % Show Material materials with Elongation of 110 % | H32 | Elongation in 50 mm | ||

260 °C | 80 % Show Material materials with Elongation of 80 % | H32 | Elongation in 50 mm | ||

205 °C | 45 % Show Material materials with Elongation of 45 % | H32 | Elongation in 50 mm | ||

150 °C | 37 % Show Material materials with Elongation of 37 % | H32 | Elongation in 50 mm | ||

100 °C, 0 °C | 20 % Show Material materials with Elongation of 20 % | H32 | Elongation in 50 mm | ||

24 °C | 18 % Show Material materials with Elongation of 18 % | H32 | Elongation in 50 mm | ||

-80 °C | 23 % Show Material materials with Elongation of 23 % | H32 | Elongation in 50 mm | ||

-195 °C | 32 % Show Material materials with Elongation of 32 % | H32 | Elongation in 50 mm | ||

Hardness, Brinell | 73.0 [-] Show Material materials with Hardness, Brinell of 73.0 [-] | H32 | AA Standards | ||

73.0 [-] Show Material materials with Hardness, Brinell of 73.0 [-] | H32 | 500 kg load, 10 mm ball | |||

Plane-Strain Fracture Toughnes | 22.0 - 35.0 MPa·√m Show Material materials with Plane-Strain Fracture Toughnes of 22.0 - 35.0 MPa·√m | Typical for Wrought 5000 Series Aluminium | |||

Poisson's ratio | 0.33 [-] Show Material materials with Poisson's ratio of 0.33 [-] | Typical for Wrought 5000 Series Aluminium | |||

Shear modulus | 26.0 - 26.5 GPa Show Material materials with Shear modulus of 26.0 - 26.5 GPa | Typical for Wrought 5000 Series Aluminium | |||

Shear strength | 165.0 MPa Show Material materials with Shear strength of 165.0 MPa | H32 | |||

Tensile strength | 275.0 MPa Show Material materials with Tensile strength of 275.0 MPa | H32 | AA Standards | ||

250.0 - 305.0 MPa Show Material materials with Tensile strength of 250.0 - 305.0 MPa | H32 | AA Standards, ASTM B209, ASTM B547 | |||

250.0 MPa Show Material materials with Tensile strength of 250.0 MPa | H32 | AA Standards, ASTM B234 | |||

270.0 MPa Show Material materials with Tensile strength of 270.0 MPa | H32 | ||||

370 °C | 40 MPa Show Material materials with Tensile strength of 40 MPa | H32 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | ||

315 °C | 75 MPa Show Material materials with Tensile strength of 75 MPa | H32 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | ||

260 °C | 117 MPa Show Material materials with Tensile strength of 117 MPa | H32 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture | ||

205 °C | 172 MPa Show Material materials with Tensile strength of 172 MPa | H32 | |||

150 °C | 220 MPa Show Material materials with Tensile strength of 220 MPa | H32 | |||

100 °C | 270 MPa Show Material materials with Tensile strength of 270 MPa | H32 | |||

24 °C | 275 MPa Show Material materials with Tensile strength of 275 MPa | H32 | |||

0 °C | 283 MPa Show Material materials with Tensile strength of 283 MPa | H32 | |||

-80 °C | 290 MPa Show Material materials with Tensile strength of 290 MPa | H32 | |||

-195 °C | 407 MPa Show Material materials with Tensile strength of 407 MPa | H32 | |||

Unlock all property charts | |||||

Yield strength | 205.0 MPa Show Material materials with Yield strength of 205.0 MPa | H32 | AA Standards | RP02 | |

180.0 MPa Show Material materials with Yield strength of 180.0 MPa | H32 | AA Standards, ASTM B209, ASTM B234, ASTM B547 | RP02 | ||

371 °C | 29 MPa Show Material materials with Yield strength of 29 MPa | H32 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | ||

316 °C | 50 MPa Show Material materials with Yield strength of 50 MPa | H32 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | ||

260 °C | 75 MPa Show Material materials with Yield strength of 75 MPa | H32 | up to 10000 h at temperature, at 35 MPa/min to yield strength and then at strain rate of 5%/min to fracture, RP02 | ||

204 °C | 130 MPa Show Material materials with Yield strength of 130 MPa | H32 | |||

149 °C | 180 MPa Show Material materials with Yield strength of 180 MPa | H32 | |||

100 °C | 200 MPa Show Material materials with Yield strength of 200 MPa | H32 | |||

24 °C, -28 °C | 205 MPa Show Material materials with Yield strength of 205 MPa | H32 | |||

-80 °C | 215 MPa Show Material materials with Yield strength of 215 MPa | H32 | |||

-196 °C | 250 MPa Show Material materials with Yield strength of 250 MPa | H32 | |||

210.0 MPa Show Material materials with Yield strength of 210.0 MPa | H32 | ||||

Unlock all property charts |

Thermal

Property | Value | Condition | Comment |
---|---|---|---|

Coefficient of thermal expansion | 2.4e-05 1/K Show Material materials with Coefficient of thermal expansion of 2.4e-05 1/K | H32 | |

Max service temperature | 150.0 °C Show Material materials with Max service temperature of 150.0 °C | Typical for Wrought 5000 Series Aluminium | |

Melting point | 600.0 °C Show Material materials with Melting point of 600.0 °C | H32 | |

Specific heat capacity | 900.0 J/(kg·K) Show Material materials with Specific heat capacity of 900.0 J/(kg·K) | H32 | |

Thermal conductivity | 130.0 W/(m·K) Show Material materials with Thermal conductivity of 130.0 W/(m·K) | H32 |

Electrical

Property | Value | Comment |
---|---|---|

Electrical conductivity | 18000000.0 - 31000000.0 S/m Show Material materials with Electrical conductivity of 18000000.0 - 31000000.0 S/m | Typical for Wrought 5000 Series Aluminium |

Electrical resistivity | 3.3e-08 - 5e-08 Ω·m Show Material materials with Electrical resistivity of 3.3e-08 - 5e-08 Ω·m | Typical for Wrought 5000 Series Aluminium |

Chemical properties

Property | Value | Condition | Related Standards |
---|---|---|---|

Aluminium | 94.5 - 97.1 % Show Material materials with Aluminium of 94.5 - 97.1 % | H32 | |

Chromium | 0.05 - 0.2 % Show Material materials with Chromium of 0.05 - 0.2 % | H32 | AA Standards, ASTM B209, ASTM B234, ASTM B547 |

Copper | 0.1 % Show Material materials with Copper of 0.1 % | H32 | AA Standards, ASTM B209, ASTM B234, ASTM B547 |

Iron | 0.40 % Show Material materials with Iron of 0.40 % | H32 | AA Standards, ASTM B209, ASTM B234, ASTM B547 |

0.4 % Show Material materials with Iron of 0.4 % | H32 | ||

Magnesium | 2.4 - 3.0 % Show Material materials with Magnesium of 2.4 - 3.0 % | H32 | AA Standards, ASTM B209, ASTM B234, ASTM B547 |

Manganese | 0.5 - 1.0 % Show Material materials with Manganese of 0.5 - 1.0 % | H32 | AA Standards, ASTM B209, ASTM B234, ASTM B547 |

Other | 0.15 % Show Material materials with Other of 0.15 % | H32 | |

Silicon | 0.25 % Show Material materials with Silicon of 0.25 % | H32 | AA Standards, ASTM B209, ASTM B234, ASTM B547 |

Titanium | 0.2 % Show Material materials with Titanium of 0.2 % | H32 | AA Standards, ASTM B209, ASTM B234, ASTM B547 |

Zinc | 0.25 % Show Material materials with Zinc of 0.25 % | H32 | AA Standards, ASTM B209, ASTM B234, ASTM B547 |

Technological properties

Property | ||
---|---|---|

Brazing | general: no brazing is known or developed | |

Corrosion properties | Stress corrosion cracking: no damage during operation and laboratory tests, general: very good, without protection in industrial or seawater atmosphere | |

General machinability | General: poor (O, H32, H111), sufficient (H34) | |

Workability | general (condition): good (O), acceptable (H32, H34, H111) |